 dimension $n$ and proves [@Pro88 Proposition 3.1] that the indecomposable trace free tensor character is also given by the identity (\[eq:SymplecticCharacter\]) with $N=\frac{n+1}{2}$.

As in the previous case, we give a combinatorial interpretation in terms of symplectic patterns. Let $n$ be odd and define the weight of an $n$-symplectic pattern $P$ as $$w_{odd}(P)=x_{\frac{n+1}{2}}^{R_n-R_{n-1}} \prod_{i=1}^{\frac{n-1}{2}} x_i^{R_{2i}-2R_{2i-1}+R_{2i-2}}.$$

It holds true [@Pro94 Theorem 4.2] that the generating function of all $n$-symplectic patterns with top row $\lambda$ with respect to the weight function $w_{odd}$ is given by the symplectic character $sp_{\lambda} (x_1,\dots,x_{\frac{n+1}{2}})$. This implies $$sp_{(K-k_1,\dots,K-k_{\frac{n+1}{2}})} (1,\dots,1)
    = \prod_{1\leq i<j\leq \frac{n+1}{2}}\frac{(k_j-k_i+j-i)(2K+n+2-k_j-k_i-j-i)}{(j-i)(j+i-1)}.$$

[^1]: Supported by the Austrian Science Foundation FWF, START grant Y463 and SFB grant F50.
 ---
abstract: 'In oxide materials, nanostructuring effect has been found very promising approach for the enhancement of *figure-of-merit*, *ZT*. In the present work, we have synthesized La$_{0.7}$Sr$_{0.3}$MnO$_{3}$ (LSMO) compound using sol-gel method and samples of crystallite size of $\sim$20, $\sim$41, and $\sim$49 nm were obtained by giving different heat treatment. Seebeck coefficient ($\alpha$), electrical resistivity ($\rho$), and thermal conductivity ($\kappa$) measurements were carried out in 300-600 K temperature range. The systematic change in the values of $\alpha$ from $\sim$ -19 $\mu$V/K to $\sim
dimension   $ n$ and proves [ @Pro88 Proposition 3.1 ] that the indecomposable trace free tensor fictional character is besides given by the identity (\[eq: SymplecticCharacter\ ]) with $ N=\frac{n+1}{2}$. 

 As in the previous subject, we hold a combinatorial interpretation in condition of symplectic patterns. Let $ n$ be curious and define the weight of an $ n$-symplectic convention   $ P$ as $ $ w_{odd}(P)=x_{\frac{n+1}{2}}^{R_n - R_{n-1 } } \prod_{i=1}^{\frac{n-1}{2 } } x_i^{R_{2i}-2R_{2i-1}+R_{2i-2}}.$$ 

 It holds true [ @Pro94 Theorem   4.2 ] that the generating routine of all $ n$-symplectic traffic pattern with top row   $ \lambda$ with respect to the weight function   $ w_{odd}$ is given by the symplectic fictional character $ sp_{\lambda } (x_1,\dots, x_{\frac{n+1}{2}})$. This implies $ $ sp_{(K - k_1,\dots, K - k_{\frac{n+1}{2 } }) } (1,\dots,1) 
     = \prod_{1\leq i < j\leq \frac{n+1}{2}}\frac{(k_j - k_i+j - i)(2K+n+2 - k_j - k_i - j - i)}{(j - i)(j+i-1)}.$$ 

 [ ^1 ]: Supported by the Austrian Science Foundation FWF, START grant Y463 and SFB accord F50. 
  --- 
 abstract:' In oxide materials, nanostructuring effect has been found very promising access for the enhancement of * figure - of - merit *, * ZT *. In the present work, we have synthesized La$_{0.7}$Sr$_{0.3}$MnO$_{3}$ (LSMO) compound using sol - gelatin method and samples of crystallite size of $ \sim$20, $ \sim$41, and $ \sim$49 nm were obtained by giving different heat discussion. Seebeck coefficient ($ \alpha$), electric electric resistance ($ \rho$), and thermal conductivity ($ \kappa$) measurements were carried out in 300 - 600 K temperature range. The systematic change in the value of $ \alpha$ from $ \sim$ -19 $ \mu$V / kelvin to $ \sim
 dilension $n$ and proves [@Pro88 Kroposition 3.1] that the invecompoaable trxce free tensor character is aoso guven by the identity (\[ed:SymplectpcCharactwr\]) wmth $N=\frac{n+1}{2}$.

As in vge prevljus dwse, ce give a combinstorial inderpretation it gexms of symplectic patterns. Let $n$ be jdd and dffine the weigrt og an $h$-symplectic pattern $P$ as $$w_{odd}(P)=x_{\frac{h+1}{2}}^{R_n-R_{n-1}} \pgod_{i=1}^{\frac{n-1}{2}} x_i^{R_{2i}-2R_{2i-1}+R_{2o-2}}.$$

It holds true [@Pro94 Theorem 4.2] thah the generating fknction of qll $g$-wymplectic pxtterns wiuh top row $\lajbda$ with respect to the weight funccion $w_{odd}$ is guvej by the sym'lectib character $si_{\kambda} (x_1,\dots,x_{\grac{n+1}{2}})$. This impkiev $$sp_{(K-k_1,\dots,K-k_{\frac{n+1}{2}})} (1,\dots,1)
    = \prod_{1\leq i<j\leq \ftac{n+1}{2}}\frac{(k_j-n_i+l-i)(2K+n+2-k_j-k_i-j-i)}{(j-i)(j+i-1)}.$$

[^1]: Supporree by jhe Agstrkqn Rcitncx Fkundatlon FWF, START grant Y463 ane SFB grant F50.
 ---
abstrsce: 'In oxide matsrials, nwnostructuring effect has been found vegy pdomising approach for tye enhancement of *figore-of-merit*, *ZT*. In the present work, we have synthesized La$_{0.7}$Sr$_{0.3}$MtO$_{3}$ (LSJU) cimiouna uding sol-gel method and samples of crystallite aiee pf $\sim$20, $\sim$41, and $\sim$49 nm werr lbywined by givivg difysrsnt heat treatment. Seebech coedficient ($\wlphs$), electrical resistivity ($\rhi$), and thermaj conductivity ($\kappc$) measuremencs werg carroed out in 300-600 K temperatuxe ranfe. The systfmatic chzvge in the valuer on $\anpha$ from $\sim$ -19 $\mu$V/K to $\sim
dimension $n$ and proves [@Pro88 Proposition 3.1] indecomposable free tensor is also given $N=\frac{n+1}{2}$. in the previous we give a interpretation in terms of symplectic patterns. $n$ be odd and define the weight of an $n$-symplectic pattern $P$ as \prod_{i=1}^{\frac{n-1}{2}} x_i^{R_{2i}-2R_{2i-1}+R_{2i-2}}.$$ It holds true [@Pro94 Theorem 4.2] that the generating function of $n$-symplectic with row with respect to the weight function $w_{odd}$ is given by the symplectic character $sp_{\lambda} (x_1,\dots,x_{\frac{n+1}{2}})$. This $$sp_{(K-k_1,\dots,K-k_{\frac{n+1}{2}})} (1,\dots,1) = \prod_{1\leq i<j\leq \frac{n+1}{2}}\frac{(k_j-k_i+j-i)(2K+n+2-k_j-k_i-j-i)}{(j-i)(j+i-1)}.$$ [^1]: Supported the Austrian Science Foundation START grant Y463 and SFB F50. abstract: 'In materials, effect been found very approach for the enhancement of *figure-of-merit*, *ZT*. In the present work, we have synthesized La$_{0.7}$Sr$_{0.3}$MnO$_{3}$ (LSMO) compound sol-gel method of crystallite of $\sim$41, $\sim$49 nm were giving different heat treatment. Seebeck coefficient ($\rho$), and thermal conductivity ($\kappa$) measurements were carried in 300-600 temperature range. The systematic change in values of $\alpha$ from $\sim$ -19 $\mu$V/K to
 dimension $n$ and proves [@Pro88 ProPosition 3.1] thAt the IndEcoMpOsabLe trAce free tensor cHAracTer is also given by the ideNtity (\[Eq:sYmplECtIcChaRacter\]) wITh $n=\FRac{N+1}{2}$.

AS iN thE pREvIous cAse, We give a CombinatorIal InTerpretation IN tErms of sympLecTic patterns. LEt $n$ Be odd aNd DefINe the WeiGht of An $n$-symPLectic Pattern $P$ aS $$w_{ODd}(P)=x_{\frAC{n+1}{2}}^{R_n-R_{n-1}} \pROD_{i=1}^{\Frac{N-1}{2}} x_i^{R_{2i}-2R_{2i-1}+R_{2i-2}}.$$

It holds tRUe [@pRo94 Theorem 4.2] that tHe geneRaTInG FUncTioN of all $n$-symPlEctic PAtterns WItH TOP roW $\Lambda$ with resPect to the weIGht FunctiOn $W_{odD}$ Is giveN by thE sYMplEctic characTer $sP_{\lambda} (x_1,\dOts,x_{\frAC{n+1}{2}})$. This iMPlies $$sp_{(k-k_1,\dots,k-k_{\fRac{N+1}{2}})} (1,\dotS,1)
    = \PrOd_{1\Leq I<j\LEq \fRAc{N+1}{2}}\frAC{(k_j-K_i+j-i)(2K+n+2-k_j-K_i-J-i)}{(J-i)(j+i-1)}.$$

[^1]: SUppoRTED By thE AuStriAn SciEnce FoundatioN FWf, STArt grAnt Y463 aNd SFB GranT F50.
 ---
AbstrAct: 'In oXide mAtErials, nanostrucTuriNg effect hAs bEeN foUnD very PRomisiNg aPprOach for The enhaNCemEnT OF *FiGure-of-merit*, *ZT*. In the PrESEnT work, we hAve synTHeSiZEd La$_{0.7}$Sr$_{0.3}$Mno$_{3}$ (LsMO) CompOUNd usiNg soL-GeL method aNd sampLEs Of CrystalLiTe size Of $\Sim$20, $\Sim$41, And $\siM$49 Nm weRe obtaIned by giVing dIFferent heat treATment. Seebeck cOEfFICiENt ($\alPha$), Electrical rEsisTIvitY ($\rho$), ANd TheRMal coNductIvITy ($\KAppa$) measurements werE cArried Out in 300-600 k temperature rAnge. The sysTEMAtic chanGe in THe VAlues of $\alpha$ frOm $\sim$ -19 $\Mu$V/K to $\sim
 dimension $n$ and proves[@Pro88 Pr oposi tio n 3 .1 ] th at t he indecomposa b le t race free tensor chara cteris also gi ven b y the i d en t i ty(\ [e q:S ym p le cticC har acter\] ) with $N= \fr ac {n+1}{2}$.
A sin the pre vio us case, wegiv e a co mb ina t orial  in terpr etatio n  in te rms of sy mp l ecticp atterns . Le t $n $ be odd and defi n et he weight of a n $n$- sy m pl e c tic  pa ttern $P$as  $$w_ { odd}(P) = x_ { \ f rac { n+1}{2}}^{R_n -R_{n-1}} \ p rod _{i=1} ^{ \fr a c{n-1} {2}}x_ i ^{R _{2i}-2R_{2 i-1} +R_{2i-2} }.$$
I t holds true [@ Pro94The ore m 4. 2 ]th atth e  ge n er ati n g f unctionof  a ll $n $-sy m p l e ctic  pa tter ns wi th top row $\ lam bda$ wit h res pectto t he  weig ht fun ction  $ w_{odd}$ is giv en b y the sym ple ct icch aract e r $sp_ {\l amb da} (x_ 1,\dots , x_{ \f r a c {n +1}{2}})$. This im pl i e s$$sp_{(K -k_1,\ d ot s, K -k_{\fra c{ n+1 }{2} } ) } (1, \dot s ,1 )
    =\prod_ { 1\ le q i<j\l eq  \frac {n +1} {2} }\fra c {(k_ j-k_i+ j-i)(2K+ n+2-k _ j-k_i-j-i)}{(j - i)(j+i-1)}.$$ 
[ ^ 1 ]: Supp ort ed by the A ustr i an S cien c eFou n datio n FWF ,S TA R T grant Y463 and SF BgrantF50. ---
abstract : 'In oxid e m aterials , na n os t ructuring effe ct ha s been fou n d very p romis ing appr oach fort h e enhanc eme ntof*fi g u re -of-merit*, * Z T *. I nthe pre sen t work,  we  ha vesyn th esized La $_{0.7}$ Sr $_ {0 .3 }$M nO$_{ 3 }$ (LSMO )com po und  usin g  sol-g el me thod  a nd sam ples of cr y s tall it esize  of  $ \sim$ 20,$ \si m$41, a nd $\sim$ 49n m we re  o btained  by giving di ff erent heat  t rea tment. S eebeck c oefficient ($\alpha$),e lectric alresis tivi ty ($\rho $),  and t her m al con ductiv ity ( $\ kap p a $) me a s ur eme nt s were car r i edout i n300- 600 K t emperature range.T hesystematic ch ang e in t he  va l ue s  of  $ \ alp h a $ from $\sim$ - 19 $\mu$V/ Kt o$\sim
 dimension $n$_and proves_[@Pro88 Proposition 3.1] that_the indecomposable_trace_free tensor_character_is also given_by the identity_(\[eq:SymplecticCharacter\]) with $N=\frac{n+1}{2}$.

As in_the previous case,_we_give a combinatorial interpretation in terms of symplectic patterns. Let $n$ be odd and_define_the weight_of_an_$n$-symplectic pattern $P$ as $$w_{odd}(P)=x_{\frac{n+1}{2}}^{R_n-R_{n-1}} \prod_{i=1}^{\frac{n-1}{2}}_x_i^{R_{2i}-2R_{2i-1}+R_{2i-2}}.$$

It holds true [@Pro94 Theorem 4.2]_that the_generating function of all $n$-symplectic patterns with top_row $\lambda$_with respect to_the weight function $w_{odd}$ is given by the symplectic character_$sp_{\lambda} (x_1,\dots,x_{\frac{n+1}{2}})$. This implies $$sp_{(K-k_1,\dots,K-k_{\frac{n+1}{2}})} (1,\dots,1)
_  _=_\prod_{1\leq_i<j\leq \frac{n+1}{2}}\frac{(k_j-k_i+j-i)(2K+n+2-k_j-k_i-j-i)}{(j-i)(j+i-1)}.$$

[^1]: Supported by_the Austrian Science Foundation FWF, START_grant Y463 and SFB grant F50.
_---
abstract: 'In oxide materials, nanostructuring effect has_been found very promising approach for_the enhancement of *figure-of-merit*, *ZT*._In the_present work, we have synthesized_La$_{0.7}$Sr$_{0.3}$MnO$_{3}$ (LSMO) compound_using sol-gel_method and samples_of crystallite size of $\sim$20, $\sim$41,_and $\sim$49 nm_were obtained by giving different heat_treatment._Seebeck coefficient ($\alpha$),_electrical_resistivity_($\rho$), and_thermal conductivity ($\kappa$)_measurements_were carried_out_in 300-600 K temperature range. The_systematic_change in the values of $\alpha$ from_$\sim$ -19 $\mu$V/K to_$\sim